- Solid solution strengthening
Solid solution strengthening is a type of
alloying that can be used to improve the strength of a pure metal. The technique works by adding atoms of one element (the alloying element) to the crystalline lattice another element (the base metal). The alloying element diffuses into the matrix, forming a solid solution. In most binary systems, when alloyed above a certain concentration, a second phase will form. When this increases the strength of the material, the process is known as precipitation strengthening, but this is not always the case.
Depending on the size of the alloying element, a
substitutional solid solutionor an interstitial solid solutioncan form. In both cases, the overall crystal structure is essentially unchanged.
Substitutional solid solution strengthening occurs when the solute atom is large enough that it can replace solvent atoms in their lattice positions. According to the
Hume-Rothery rules, solvent and solute atoms must differ in atomic sizeby less than 15% in order to form this type of solution. Because both elements exist in the same crystalline lattice, both elements in their pure form must be of the same crystal structure. Examples of substitutional solid solutions include the Cu-Ni and the Ag-Au FCC binary systems, and the Mo-W BCC binary system.
When the solute atom is much smaller than the solvent atoms, an interstitial solid solution forms. This typically occurs when the solute atoms are less than half as small as the solvent atoms. The smaller solute atom essentially "crowds" into the spacings within the lattice structure, causing defects in the material. Elements commonly used to form interstitial solid solutions include H, N, C, and O. Carbon in iron (steel) is one example of interstitial diffusion.
The strength of a material is dependent on how easily dislocations in its crystal lattice can be propagated. These dislocations create stress fields within the material depending on their character. When solute atoms are introduced, local stress fields are formed that interact with those of the dislocations, impeding their motion and causing an increase in the
yield stressof the material, which means an increase in strength of the material. This gain is a result of both lattice distortion and the modulus effect.
When solute and solvent atoms differ in size, local stress fields are created (if solute atom size is larger than solvent atom size, this field is compressive, and similarly, when solute atoms are smaller than solvent atoms, this field is tensile). Depending on their relative locations, solute atoms will either attract or repel dislocations in their vicinity. This is known as the
size effect. This allows the solute atoms to relieve either tensile or compressive strain in the lattice, which in turn puts the dislocation in a lower energy state. In substitutional solid solutions, these stress fields are spherically symmetric, meaning they have no shear stress component. As such, substitutional solute atoms do not interact with the shear stress fields characteristic of screw dislocations. Conversely, in interstitial solid solutions, solute atoms cause a tetragonal distortion, generating a shear field that can interact with both edge, screw, and mixed dislocations. The attraction or repulsion of the dislocation centers to the solute particles increase the stress it takes to propagate the dislocation in any other direction. Increasing the applied stress to move the dislocation increases the yield strength of the material.
The energy density of a
dislocationis dependent on its Burgers vectoras well as the modulus of the local atoms. When the modulus of solute atoms differs from that of the host element, the local energy around the dislocation is changed, increasing the amount of force necessary to move past this energy well. This is known as the modulus effect. Meanwhile, in the specific case of a lattice distortion, the difference in lattice parameter leads to a high stress field around that solute atom that impedes dislocation movement.
Surface carburizing, or
case hardening, is one example of solid solution strengthening in which the density of solute carbon atoms is increased close to the surface of the steel, resulting in a gradient of carbon atoms throughout the material. This provides superior mechanical properties to the surface of the steel.
Solid solution strengthening increases yield strength of the material by increasing the stress to move dislocations:
where "c" is the concentration of the solute atoms, "G" is the shear modulus, "b" is the magnitude of the Burger's vector, and is the lattice strain due to the solute. This is composed of two terms, one describing lattice distortion and the other local modulus change.
Here, is the lattice distortion term, a constant dependent on the solute atoms and the term that captures the local modulus change.
The lattice distortion term can be described as:
, where "a" is the lattice parameter of the material.
Meanwhile, the local modulus change is captured in the following expression:
, where "G" is shear modulus of the solute material,
In order to achieve noticeable material strengthening via solute solution strengthening one should alloy with solutes of higher shear modulus, hence increasing the local shear modulus in the material. In addition, one should alloy with elements of different equilibrium lattice constants. The greater the different in lattice parameter, the higher the local stress fields introduced by alloying. Alloying with elements of higher shear modulus or of very different lattice parameters will increase the stiffness and introduce local stress fields respectively. In either case, the dislocation propagation will be hindered at these sites, impeding plasticity and increasing yield strength proportionally with solute concentration.
Solid solution strengthening depends on: - Concentration of solute atoms - Shear modulus of solute atoms - Size of solute atoms - Valency of solute atoms (for ionic materials)
Nevertheless, one should not add so much solute as to precipitate a new phase. This occurs if the concentration of the solute reaches a high critical point given by the binary system phase diagram. This critical concentration therefore puts a limit to the amount of solid solution strengthening a material can have, as the material cannot be infinitely strengthened.
Strength of materials
Strengthening mechanisms of materials
* [http://www.key-to-steel.com/Articles/Art107.htm The Strengthening of Iron and Steel]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Strengthening mechanisms of materials — Methods have been devised to modify the yield strength, ductility, and toughness of both crystalline and amorphous materials. These strengthening mechanisms give engineers the ability to tailor the mechanical properties of materials to suit a… … Wikipedia
Precipitation hardening — Precipitation hardening, also called age hardening, is a heat treatment technique used to increase the yield strength of malleable materials, including most structural alloys of aluminium, magnesium, nickel and titanium, and some stainless steels … Wikipedia
Hardness — This article is about mechanical properties of materials. For other uses, see Hard. Hardness is the measure of how resistant solid matter is to various kinds of permanent shape change when a force is applied. Macroscopic hardness is generally… … Wikipedia
Precipitation (chemistry) — This article is about the chemical phenomemon. For other uses, see Precipitation. Precipitate redirects here. For the album by Interpol, see Precipitate EP. Chemical Precipitation Precipitation is the formation of a solid in a solution or inside… … Wikipedia
Strength of materials — Internal force lines are denser near the hole, a common stress concentration In materials science, the strength of a material is its ability to withstand an applied stress without failure. The applied stress may be tensile, compressive, or shear … Wikipedia
Superalloy — A superalloy, or high performance alloy, is an alloy that exhibits excellent mechanical strength and creep resistance at high temperatures, good surface stability, and corrosion and oxidation resistance. Superalloys typically have an austenitic… … Wikipedia
Brazing — This article is about the metal joining process. For the cooking technique, see braising. Brazing practice Brazing is a metal joining process whereby a filler metal is heated above and distributed between two or more close fitting parts by… … Wikipedia
Carburization — (often referred to as carburizing) is a heat treatment process which iron or steel is heated to below the melting point in the presence of a solid, liquid, or gaseous material which decomposes so as to liberate carbon when heated to the… … Wikipedia
Inconel — is a registered trademark of Special Metals Corporation that refers to a family of austenitic nickel based superalloys. Inconel alloys are typically used in high temperature applications. It is often referred to in English as Inco (or… … Wikipedia
Yield (engineering) — The yield strength or yield point of a material is defined in engineering and materials science as the stress at which a material begins to deform plastically. Prior to the yield point the material will deform elastically and will return to its… … Wikipedia